Int. J. Electrochem. Sci., 15 (2020) 5487 – 5499, doi: 10.20964/2020.06.22
International Journal of
Corrosion Inhibition of Carbon Steel in Hydrochloric Acid by
Chrysanthemum Indicum Extract
Haibing Zhang1, Zihui Ni2, Haitao Wu1, Peng Xu2, Zidong Li1, Wuyang Zhang1,
Huixian Huang1, Qing Zhou1, Xingui Yue1, Jiankang Bao1, Xueming Li2,*
1 State Grid Chongqing Electric Power Company, Chongqing 400015, China
2 School of Chemistry and Chemical Engineering, Chongqing University, Chongqing 400044, China
† Haibing Zhang and Zihui Ni contributed equally to this work.
Received: 6 January 2020 / Accepted: 20 February 2020 / Published: 10 May 2020
Biodegradable and inexpensive plant extracts are one of the most promising materials for future metal
pickling inhibitors. The corrosion inhibition performance of the Chrysanthemum indicum extract on
carbon steel in 1 mol/L hydrochloric acid solution was evaluated by potentiodynamic polarization, EIS
and SEM. Then, FTIR was applied for characterization of functional groups in the Chrysanthemum
indicum extract. Electrochemical measurement results showed that the inhibition performance of 500
mg/L extract on carbon steel at 25 oC was up to 93%. The FTIR spectra showed that the extract contained
O‒H, N‒H, C‒H, C=C, C‒N and C‒O groups, which may be the characteristic group of excellent
corrosion inhibitor. The adsorption of this inhibitor on the surface of carbon steel is Langmuir adsorption.
This study provides an experimental supplement for the applied of plant extracts as metal pickling
Keywords: corrosion inhibitor, extract, carbon steel, electrochemical test
Carbon steel is widely used in the construction of transmission towers due to its excellent
mechanical properties and low cost. Generally, the oxidation layer on the surface of the carbon steel
needs to be removed by pickling before the carbon steel is processed into transmission tower. Corrosion
inhibitors are usually used to inhibit the corrosion of carbon steel during this pickling process. However,
the traditional corrosion inhibitors are expensive, difficult to degrade and harmful to the environment
and human beings. Therefore, a great deal of efforts have been made in developing low cost, high
efficiency and environmentally friendly corrosion inhibitors.
Int. J. Electrochem. Sci., Vol. 15, 2020
The plant extraction may become corrosion inhibitors due to the advantages of wide sources and
biodegradation. It was previously reported that the extracts of Soybean , Chenopodium , Solanum
lasiocarpum , Persian Liquorice , Ginkgo , Dacryodis edulis , Tagetes erecta ,
Glycyrrhiza glabra , Corchorus olitorius , Saraca ashoka , Geissospermum , Cuscuta
reflexa , Ircinia strobilina , Primula vulgaris , Tobacco , Henna , Asparagus
racemosus , Centaurea cyanus , Ginger , Bambusa Arundinacea , Thymus vulgaris ,
Azadirachta indica [22, 23], Longan , Justicia gendarussa , Salvia officinalis [26, 27], and Ficus
tikoua  showed excellent corrosion inhibition for carbon steel in acidic medium. Heteroatoms such
as nitrogen (N), oxygen (O), sulfur (S) and phosphorus (P) can be used as adsorption centers of inhibitor
molecules, and these atoms also have become important features of efficient corrosion inhibitors. The
Chrysanthemum indicum extract contains 1,8-cineole, camphor, borneol and bornyl acetate, which
contain N, O and other heteroatoms [29-32]. Therefore, Chrysanthemum indicum extract has the
potential to be used as an inhibitor.
In this study, a powdery extract was successfully obtained from Chrysanthemum indicum by hot
water extraction and subsequent freeze‒drying process. The inhibition performance and mechanism of
the extract on carbon steel in hydrochloric acid were systematically evaluated by potentiodynamic
polarization, electrochemical impedance spectroscopy (EIS), scanning electron microscopy (SEM) and
Fourier transformed infrared spectroscopy (FTIR). In addition, the adsorption behavior of extractive
inhibitor molecules on the surface of carbon steel was analyzed in detail. This work provides an
important reference for plant extracts as corrosion inhibitors for carbon steel pickling.
2. EXPERIMENTAL DETAILS
The chemical composition (wt.%) of carbon steel employed for electrochemical experiments and
surface analysis are 0.140% C, 0.550% Mn, 0.190% Si, 0.028% P, 0.020% S, and the rest is Fe.
Specifically, carbon steel specimens with exposed surfaces of 1.0 cm × 1.0 cm and 0.5 cm × 0.5 cm ×
0.5 cm were used for electrochemical experiments and surface analysis, respectively.
For the preparation of the Chrysanthemum indicum extract, the procedure was employed
according to our previously reported. The dried Chrysanthemum indicum was immersed in deionized
water at 90 °C for 1 h, and then filtered and concentrated to dryness. Finally, the obtained brown‒black
viscous substance was freeze‒dried for 24 h and crushed into powder.
To evaluate the corrosion inhibition performance of the Chrysanthemum indicum extract in acidic
environment, the acidic solution used in this study was 1.0 mol/L HCl. All reagents used in this work
were of analytical grade and were not purified before use.
2.2 Electrochemical experiments
The inhibition performance of the Chrysanthemum indicum extract was systematically evaluated
by methods of potentiodynamic polarization and electrochemical impedance spectroscopy (EIS). The
Int. J. Electrochem. Sci., Vol. 15, 2020
electrode was stabilized in 1.0 mol/L HCl solution for 20 min before all electrochemical experiments to
achieve steady state. The EIS were measured in the range of 100 kHz ‒ 0.01 Hz with an amplitude of 10
mV. The EIS parameters of carbon steel were obtained by fitting with Zsimpwin software. The range of
the potentiodynamic polarization were ‒300 mV to +300 mV with a scanning rate of 1 mV/s.
The corrosion morphology of carbon steel immersed in 1.0 mol/L HCl solution without and with
the Chrysanthemum indicum extract was characterized by scanning electron microscopy. FTIR
technique over the range from 4000 to 400 cm‒1 was employed to investigate the groups in the extract.
3. RESULTS AND DISCUSSION
3.1 EIS measurements
The corrosion inhibition performance of the Chrysanthemum indicum extract was preliminarily
evaluated by EIS measurement. It is worth noting that the OCP‒T test was performed for 20 min before
all EIS measurements to make the carbon steel electrode reach steady state. As shown in Fig. 1, the
Nyquist plots exhibit semicircle in the high frequency region.
Figure 1. Nyquist diagrams of the carbon steel electrode in hydrochloric acid solutions with 0, 20, 50,
100, 200 and 500 mg/L Chrysanthemum indicum extract
Generally, this semicircle in the high frequency region corresponds to the charge transfer
resistance (Rct) and the double‒layer capacitance (Cdl). It is because of the rough surface of the sample
or the adsorption of the inhibitor molecules that Nyquist plot appears incomplete semicircle, which is
often referred as the frequency dispersion effect. Besides, the diameter of the semicircle in Fig. 1
increases with the increase of the concentration of the corrosion inhibitor, but its shape does not change
Int. J. Electrochem. Sci., Vol. 15, 2020
significantly. Therefore, we conclude that inhibitor molecules form an adsorption film on the surface of
carbon steel to suppress the corrosion of carbon steel. However, this adsorption film does not change the
corrosion mechanism of carbon steel in hydrochloric acid solution, and the entire corrosion process is
still controlled by the charge transfer process. Finally, the diameter of the semicircle reached the
maximum with the inhibitor content was 500 mg/L, indicating that the best inhibitor performance was
achieved at 500 mg/L.
The impedance data of carbon steel in hydrochloric acid solution was fitted by Zsimpwin
software. The equivalent circuit is shown in Fig. 2. The obtained electrochemical parameters are listed
in Table 1. Here, Rs is the solution resistance, Rct is the charge transfer resistance, CPE is the constant
phase angle element, and CPE represents the double‒layer capacitance (Cdl). The definition of CPE is
where Y0 is the modulus of the CPE, w is the angular frequency, j is the imaginary number (j
‒1), and n is the dispersion effect index, which reflects the heterogeneity of the electrode surface. When
n = 0, CPE means resistance, n = ‒1, it is inductance, and n = 1, it is capacitance.
The value of Cdl can be calculated by the following equation :